]. On the one hand such an effect of doping is not to be expected in the case of a high-$T$ peak originating from optical phonons, since the lattice impurities induced by the Sr-ions are similar to the Eu-impurities discussed above. On the other hand the strong frustration of antiferromagnetism upon doping of mobile holes (cf. Ref. [@Hucker02] and references therein) would provide for a satisfying explanation for the suppression of a peak of magnetic origin. Note in this context that Eu-doping leaves the CuO$_2$-planes and therefore the magnetism almost unaffected. Hence we conclude, that the high-$T$ peak of $\kappa_{ab}$ originates from magnetic excitations which propagate only within the CuO$_2$-planes. $\kappa_{ab}$ therefore consists of a usual phonon background and a magnon contribution $\kappa_{\mathrm{mag}}$ while $\kappa_c$ is purely phononic.

Upon applying a magnetic field of 8 T no significant changes of $\kappa$ were detected. This is, however, consistent with a magnetic origin of the high-$T$ peak since the corresponding Zeeman-energy is orders of magnitude smaller than the magnetic exchange coupling $J$.

In order to extract $\kappa_{\mathrm{mag}}$ from $\kappa_{ab}$ we make use of the anisotropy of $\kappa$ assuming that the phononic part $\kappa_{ab,\mathrm {ph}}$ of $\kappa_{ab}$ is roughly proportional to $\kappa_c$ which is justified by only weakly anisotropic elastic constants [@Pintschovius91]. Since the magnetic contributions roughly follow a $T^2$-law (see below) they are expected to be negligible in the range of the low-$T$ peak. Therefore, for $\rm
La_2CuO_4$ as well as for $\rm La_{1.8}Eu_{0.2}CuO_{4}$ a reasonable estimate of $\kappa_{ab,\mathrm {ph}}$ is achieved by scaling the corresponding data for $\kappa_c$ such as to match its low-$T$ peaks with that of $\kappa_{ab}$. In Fig. \[fig1\] the data thus obtained for $\kappa_{ab,\mathrm {ph}}$ of both compounds are represented by dashed lines. $\kappa_{\mathrm{mag}}$ was extracted by subtracting $\kappa_{ab,\mathrm {ph}}$ from $\kappa_{ab}$ (open squares in Fig. \[fig1\]). This procedure involves significant
]. On the one hand such an effect of doping is not to be expected in the case of a high-$T$ acme originate from optical phonons, since the lattice impurities induce by the Sr - ions are similar to the Eu - impurity hash out above. On the other hired hand the strong frustration of antiferromagnetism upon doping of mobile hole (cf. Ref.   [ @Hucker02 ] and references therein) would put up for a hearty explanation for the suppression of a peak of magnetic origin. Note in this context that Eu - doping entrust the CuO$_2$-planes and therefore the magnetism almost unaffected. therefore we conclude, that the high-$T$ peak of $ \kappa_{ab}$ originates from charismatic excitations which circulate only within the CuO$_2$-planes. $ \kappa_{ab}$ consequently consists of a usual phonon background and a magnon contribution $ \kappa_{\mathrm{mag}}$ while $ \kappa_c$ is purely phononic. 

 Upon apply a magnetic field of 8   T no significant changes of $ \kappa$ were detect. This is, however, reproducible with a magnetic origin of the high-$T$ peak since the corresponding Zeeman - energy is orders of magnitude smaller than the magnetic central coupling $ J$. 

 In order to excerpt $ \kappa_{\mathrm{mag}}$ from $ \kappa_{ab}$ we seduce use of the anisotropy of $ \kappa$ assuming that the phononic part $ \kappa_{ab,\mathrm { ph}}$ of $ \kappa_{ab}$ is approximately proportional to $ \kappa_c$ which is justified by merely weakly anisotropic elastic constants [ @Pintschovius91 ]. Since the charismatic contributions roughly follow a $ T^2$-law (see below) they are expected to be negligible in the range of the low-$T$ peak. Therefore, for $ \rm 
 La_2CuO_4 $ as well as for $ \rm La_{1.8}Eu_{0.2}CuO_{4}$ a reasonable estimate of $ \kappa_{ab,\mathrm { ph}}$ is achieve by scaling the represent datum for $ \kappa_c$ such as to pit its low-$T$ peaks with that of $ \kappa_{ab}$. In Fig. \[fig1\ ] the data thus prevail for $ \kappa_{ab,\mathrm { ph}}$ of both compounds are represented by dashed line. $ \kappa_{\mathrm{mag}}$ was extracted by subtracting $ \kappa_{ab,\mathrm { ph}}$ from $ \kappa_{ab}$ (open squares in Fig. \[fig1\ ]). This routine involves meaning
]. On the one hand such an efnect of doping is not tm be espected kn the case of a high-$T$ peak lruginaupng from optical phonuns, since the latrice umpurities induced by ths Sr-imis are similar jo the Eu-impgrities discusvea cbove. On the other hand the strong fwustratooj of antiferroiagnttifm ulon doping of mobile holes (cf. Ref. [@Hhcker02] aid references tnerein) would provide for a satlsfying explanatioj for the solprqwsion of a pdak of magnetic origin. Note in this context that Eu-dooing keaves the CyO$_2$-ppdnes and thxreforv the magnetism almosd unaffrcted. Hence we coicluee, that the high-$T$ pean of $\kappa_{ab}$ origigates frok jagnetic excitatiinw whiwh psopaeqte onmy wjthin hhe CuO$_2$-planes. $\kappa_{ab}$ thwrefore consists of a lxual phonon gackgrjugd and a magnon contribution $\kappa_{\mathrk{maf}}$ while $\kappa_c$ is purelt phononic.

Upon applyijg a magnqtic field of 8 T no significant changes of $\kappa$ ware dxtdcttd. This us, however, consistent with a magnetic origin of fht hpgh-$T$ peak since tme corresponding Zrelam-gnergy is ordets of mcfnjtude smaller than the madnetix exchangt coulling $J$.

In order to extract $\jappa_{\mathrm{mcg}}$ drom $\kappa_{ab}$ we mane use of tke anixotroly of $\kappa$ assuming thct the phononic pwrt $\kappa_{zc,\mathrm {ph}}$ of $\kaopa_{sb}$ is roughly proportional tj $\kappa_c$ xhich is jusgifigd by ogly weakly anisotropic elastic condtantd [@[intschoviks91]. Since the magnetic contributmpns roughly gonlof a $T^2$-law (see nelow) they are qxpected to be neglignble iv the rangv of the now-$T$ peak. Trerefore, for $\sl
La_2CuO_4$ as wenl as fow $\rm La_{1.8}Ey_{0.2}CuO_{4}$ a fdasonable estikate of $\kckpa_{ab,\mathrn {ph}}$ is achieved bn scaujng the correspindung data for $\kalpa_z$ stcj es to katch its lof-$T$ pdakr with that of $\kaipa_{xb}$. Im Fig. \[fig1\] the data tvus kbtained for $\kappa_{sb,\iathrm {py}}$ of botr compounds ate represented by fashev liner. $\kapla_{\mwthrm{mag}}$ was extracted by subtdacting $\kwppw_{ab,\mathrm {ph}}$ fron $\kappa_{ab}$ (opzn squares in Fig. \[fig1\]). This procedure invilves significant
]. On the one hand such an doping not to expected in the originating optical phonons, since lattice impurities induced the Sr-ions are similar to the discussed above. On the other hand the strong frustration of antiferromagnetism upon doping mobile holes (cf. Ref. [@Hucker02] and references therein) would provide for a satisfying for suppression a of magnetic origin. Note in this context that Eu-doping leaves the CuO$_2$-planes and therefore the magnetism unaffected. Hence we conclude, that the high-$T$ peak $\kappa_{ab}$ originates from magnetic which propagate only within the $\kappa_{ab}$ consists of usual background a magnon contribution while $\kappa_c$ is purely phononic. Upon applying a magnetic field of 8 T no significant changes of were detected. however, consistent a origin the high-$T$ peak corresponding Zeeman-energy is orders of magnitude magnetic exchange coupling $J$. In order to extract from $\kappa_{ab}$ make use of the anisotropy of assuming that the phononic part $\kappa_{ab,\mathrm {ph}}$ of is roughly proportional to $\kappa_c$ which is justified by only weakly anisotropic elastic constants [@Pintschovius91]. magnetic contributions roughly follow $T^2$-law (see below) are to negligible the range the low-$T$ peak. Therefore, for $\rm La_2CuO_4$ as well as for La_{1.8}Eu_{0.2}CuO_{4}$ a reasonable estimate of $\kappa_{ab,\mathrm {ph}}$ is achieved by corresponding for $\kappa_c$ such to match its low-$T$ with of $\kappa_{ab}$. In Fig. data obtained of compounds represented by dashed lines. was extracted by subtracting $\kappa_{ab,\mathrm from $\kappa_{ab}$ (open squares involves significant
]. On the one hand such an effect oF doping is nOt to bE exPecTeD in tHe caSe of a high-$T$ peak ORigiNating from optical phonoNs, sinCe THe laTTiCe impUrities INdUCEd bY tHe sr-iOnS ArE simiLar To the Eu-Impurities DisCuSsed above. On tHE oTher hand thE stRong frustratIon Of antiFeRroMAgnetIsm Upon dOping oF Mobile Holes (cf. ReF. [@HUCker02] anD ReferenCES tHereIn) would provide for A SaTIsfying explanaTion foR tHE sUPPreSsiOn of a peak oF mAgnetIC origin. nOtE IN ThiS Context that Eu-Doping leaveS The cuO$_2$-plaNeS anD TherefOre thE mAGneTism almost uNaffEcted. HencE we conCLude, thaT The high-$t$ peak oF $\kaPpa_{Ab}$ orIGiNaTes FrOM maGNeTic EXciTations wHiCh PropaGate ONLY WithIn tHe Cuo$_2$-planEs. $\kappa_{ab}$ therEfoRe coNSisTs of a Usual PhonOn BackgRound aNd a maGnOn contribution $\kAppa_{\Mathrm{mag}}$ WhiLe $\KapPa_C$ is puREly phoNonIc.

UPon applYing a maGNetIc FIELd Of 8 T no significant chAnGES oF $\kappa$ weRe deteCTeD. THIs is, howeVeR, coNsisTENt witH a maGNeTic origiN of the HIgH-$T$ Peak sinCe The corReSpoNdiNg ZeeMAn-enErgy is Orders of MagniTUde smaller than THe magnetic excHAnGE CoUPlinG $J$.

IN order to extRact $\KAppa_{\MathRM{mAg}}$ fROm $\kapPa_{ab}$ wE mAKe USe of the anisotropy of $\KaPpa$ assUming That the phononIc part $\kappA_{AB,\Mathrm {ph}}$ Of $\kaPPa_{AB}$ is roughly propOrtioNal to $\kappa_C$ Which is jUstifIed by onlY weakly anISOtropic eLasTic ConStaNTS [@PIntschovius91]. SiNCE the MaGnetic cOntRibutioNs rOugHly FolLoW a $T^2$-law (see Below) theY aRe ExPeCteD to be NEgligiblE iN thE rAngE of thE Low-$T$ peAk. TheRefoRe, FoR $\Rm
LA_2CuO_4$ as wELl AS For $\rM LA_{1.8}EU_{0.2}CuO_{4}$ A reAsOnablE estIMatE of $\kappA_{ab,\mathrm {Ph}}$ iS AchiEvEd By scaliNg the correspoNdIng data for $\KaPpa_C$ such aS TO match itS low-$T$ peaks with that of $\kapPA_{ab}$. In FiG. \[fiG1\] the dAta tHus obtainEd fOr $\kappA_{ab,\MAthrm {pH}}$ of botH compOuNds ARE reprESEnTed By Dashed lineS. $\KAppA_{\mathRm{Mag}}$ wAs extraCted by subtracting $\kAPpa_{Ab,\mathrm {ph}}$ froM $\kaPpa_{aB}$ (OPeN sqUArES in fiG. \[Fig1\]). tHIs procedure invoLves signifIcANt
]. On the one hand such an  effect of  dopi ngisno t to  beexpected in th e  cas e of a high-$T$ peak o rigin at i ng f r om  opti cal pho n on s ,  si nc ethe  l a tt ice i mpu ritiesinduced by  th eSr-ions ares im ilar to th e E u-impurities  di scusse dabo v e. On  th e oth er han d  the s trong fru st r ationo f antif e r ro magn etism upon doping of mobile holes ( cf. Re f. [@ H u cke r02 ] and refe re ncest herein) wo u l d  pr o vide for a sa tisfying ex p lan ationfo r t h e supp ressi on ofa peak of m agne tic origi n. Not e  in thi s  contex t that  Eu -do ping le av esth e  Cu O $_ 2$- p lan es and t he re forethem a g n etis m a lmos t una ffected. Henc e w e co n clu de, t hat t he h ig h-$T$  peakof $\ ka ppa_{ab}$ origi nate s from ma gne ti c e xc itati o ns whi chpro pagateonly wi t hin  t h e Cu O$_2$-planes. $\ka pp a _ {a b}$ ther eforec on si s ts of aus ual  pho n o n bac kgro u nd  and a m agnonc on tr ibution  $ \kappa _{ \ma thr m{mag } }$ w hile $ \kappa_c $ isp urely phononic . 

Upon applyi n ga ma g neti c f ield of 8 T  nos igni fica n tcha n ges o f $\k ap p a$ were detected. This  i s, how ever,  consistent w ith a magn e t i c origin  oft he high-$T$ peaksince  the corre s pondingZeema n-energy  is order s of magni tud e s mal ler t ha n the magneti c exch an ge coup lin g $J$.
In  or der  to  e xtract $\ kappa_{\ ma th rm {m ag} }$ fr o m $\kapp a_ {ab }$  we  make use of  theanis ot ro p y o f $\kap p a$ a ssum in gthat  th ephono nicp art  $\kapp a_{ab,\ma thr m  {ph }} $of $\ka ppa_{ab}$ isro ughly prop or tio nal to $ \kappa_c $ which is justified by only we akl y ani sotr opic elas tic  const ant s  [@Pin tschov ius91 ].  Si n c e the m ag net ic  contribut i o nsrough ly  fol low a $ T^2$-law (see belo w ) t hey are expec ted  tob e  n egl i gi b lein the r ange of the low -$T$ peak.  T h er efore, for $\r mLa_2CuO _4$ aswella s for $ \rm La_{1 .8}Eu_{0. 2} CuO_ { 4 }$a reasonab le estim ate of $\ k appa_ { ab ,\mat hrm  {ph}} $isachie ved by sca lingthe co rr espond ing d at a for $\ kappa_c$ such as to mat ch its  low- $T$  peaks wi tht hat  of $\kap pa_{ ab}$. In F ig.  \[ fig1\ ] t h e dat a th u sobt a inedfor$ \kappa_{a b ,\ mat h r m{ph}}$ of b o t h  co mpoun dsa re rep rese nted by dashed li n es. $\kappa_{\ math r m {ma g}} $  was  e xtracted by su btr ac t i ng $\kap pa _{ab,\mathr m {ph}}$  f r om $\ kappa_ {ab}$(open s q u ar e s in F ig.\[f ig1\]). T his  p r ocedure  i nv o lves s igni fi cant
]. On_the one_hand such an effect_of doping_is_not to_be_expected in the_case of a_high-$T$ peak originating from_optical phonons, since_the_lattice impurities induced by the Sr-ions are similar to the Eu-impurities discussed above. On_the_other hand_the_strong_frustration of antiferromagnetism upon doping_of mobile holes (cf. Ref. [@Hucker02]_and references_therein) would provide for a satisfying explanation for_the_suppression of a_peak of magnetic origin. Note in this context that_Eu-doping leaves the CuO$_2$-planes and therefore_the magnetism almost_unaffected._Hence_we conclude, that the_high-$T$ peak of $\kappa_{ab}$ originates from_magnetic excitations which propagate only within_the CuO$_2$-planes. $\kappa_{ab}$ therefore consists of a_usual phonon background and a magnon_contribution $\kappa_{\mathrm{mag}}$ while $\kappa_c$ is_purely phononic.

Upon_applying a magnetic field of_8 T no significant_changes of_$\kappa$ were detected._This is, however, consistent with a_magnetic origin of_the high-$T$ peak since the corresponding_Zeeman-energy_is orders of_magnitude_smaller_than the_magnetic exchange coupling_$J$.

In_order to_extract_$\kappa_{\mathrm{mag}}$ from $\kappa_{ab}$ we make use_of_the anisotropy of $\kappa$ assuming that the_phononic part $\kappa_{ab,\mathrm {ph}}$_of_$\kappa_{ab}$ is roughly proportional_to $\kappa_c$ which is justified_by only weakly anisotropic elastic constants_[@Pintschovius91]. Since_the magnetic_contributions roughly follow a $T^2$-law (see below) they are expected to_be negligible in the range of_the low-$T$ peak. Therefore,_for $\rm
La_2CuO_4$_as_well as for_$\rm_La_{1.8}Eu_{0.2}CuO_{4}$ a_reasonable estimate of $\kappa_{ab,\mathrm {ph}}$ is achieved_by scaling_the corresponding data for $\kappa_c$ such_as to match its_low-$T$_peaks with that of $\kappa_{ab}$. In_Fig. \[fig1\] the data thus obtained_for $\kappa_{ab,\mathrm {ph}}$ of both_compounds_are_represented by dashed lines. $\kappa_{\mathrm{mag}}$_was extracted by subtracting $\kappa_{ab,\mathrm {ph}}$_from $\kappa_{ab}$ (open_squares in Fig. \[fig1\]). This procedure involves_significant